Oxidation of the sulphurised dolomite produced in the desulphurisation
of the gasification gases ^
Ramón Álvarez-Rodríguez , Carmen Clemente-Jul
A B S T R A C T
Calcium sulphide oxidation Gasification
Dolomite reacts with H2S to produce calcium sulphide and has been broadly investigated as a desulph-urisation agent due to its low-cost and favourable properties.
Because CaS reacts with water or water vapour in the environment to regenérate hydrogen sulphide and, therefore, disposal is problematic and the chemical cannot be uses as a landfill material. One of the methods used to make this material inert is oxidation to convert calcium sulphide into calcium sul-phate or calcium oxide.
In our study, tests were carried out using dolomite from Granada, Spain, that was previously calcined and sulphurised at high temperature with a gas similar to that produced in gasification facilities. To approximate real-scale results, a relatively large amount of substance was used for each sample (100-150 g) and the samples were used in a fixed-bed position.
The influence of different conditions, such as grain size, composition of the oxidation gas, gas velocity, bed length and temperature, was them investigated. The final solid products were characterised by X-ray diffraction and chemical analysis and the C02, S02, H2S and COS concentrations in the gases produced during oxidation were analysed by gas chromatography.
The results showed that the most influential factor was grain size and that the best oxidant was 02 mixed with nitrogen.
The presence of water vapour increases the residual concentration of CaS in the end product, but increased the CaO content
The higher the oxygen concentration and the higher the gas velocity, the lower the residual content of CaS. C02 used alone oxidises CaS to produce S02 and COS, but at very low rates. It also produces some CS2. Water vapour used alone can also oxidise the CaS to produce H2S and S02 but also at very low velocity.
At higher oxidation temperature, between 700°C and 850 °C, lesser residual CaS is obtained in the oxi-dised product.
During the gasification of coal or its blends with other alterna-tive fuels, sulphur is mainly present in the gas as hydrogen sul-phide. The sulphur compound can be eliminated prior to gas combustión in order to comply with legislation in forcé regarding polluting emissions and specially to avoid damage in turbines dur-ing power generation or gas engines. Removal of this compound also serves to reduce corrosión in general and, in the chemical industry, to avoid damaging certain catalysts.
The scrubbing of sulphur from the gas stream has been broadly studied by using different desulphuring agents, such as amines
used by Elcogas IGCC in Spain. However, this option requires low-ering the gas temperature, a step that involves energy losses.
Some sorbents capable of capturing H2S at high temperatures, including various metal compounds, have been studied [1,2]. Sor-bent regeneration without significant degradation over a certain number of cycles is very important. With this idea in mind a num-ber of Zn compounds [3-6], Mn and Cu compounds and blends [7-9], and several Fe compounds  have been studied. The main problem is the duration of a sufficient number of cycles without degradation.
Table 1 Chemical reactions. Number (1) (2) (3) (4) (5) (6) (7) (8) (9) (10) (11) (12) (13) (14) (15) (16) Reaction
H2S + CaO <-> CaS + H20( g ) CaS + 3/202 <-> CaO + S02 CaS + 2 02 <-> CaS04 CaS + C02 <-> CaO + COS CaS + 3C02 <-> CaO + 3CO + S02 CaS + 3H20 <-> CaO + 3H2 + S02 COS + 2 02 <-> C02 + S02 H2S + 3/202 «• H20 + S02 COS + H20( g ) «• H2S + C02 C02 + H2S «• COS + H20( g ) C02 + 2H2S «• CS2 + 2H20( g ) 2CaS + C02 <-> CS2 + 2CaO COS + CaS <-> CS2 + CaO CaS + 3CaS04 <-> 4CaO + 4S02 CaS + 4C02 <-> CaS04 + 4CO CaS + 2C02 <-> CaC03 + COS
AH° kj mol"'
-59.2 -458.9 -952.2 +93 +390 +266.6 - 5 5 2 -515.2 -33.6 +33.6 +68 +186.42 +93.4 +1020.8 +179.8 -419.9
Calcium oxide is effective in absorbing H2S from the gasification gases according to the reaction (1) given in Table 1.
However, a problem arises regarding how to handle this cal-cium sulphide product which reacts with water or water vapour and regenerates H2S as an inverse reaction to the sulphidisation reaction (1). This phenomenon has been investigated by some authors [21 ] who have demonstrated the reaction of the compound with the atmospheric water vapour o the superficial water, a prop-erty which makes it unsuitable for landfill material, an option that would have been the cheapest alternative.
Several methods to convert this product into a "non-hazardous" product or to obtain some use from it have been investigated. One of these involves reacting CaS with water and MDEA (Methyldieth-anolamine) to recover H2S at ambient temperature .
As calcium oxide is used as an absorbent at high temperature, research on its stabilisation at high temperature is also interesting. The majority of the studies carried out involve the oxidation of CaS. One of these attempts to recover CaO, to reuse it  preventing the sulphate formation. Unfortunately this reaction must be per-formed at very high temperatures (above 1400 °C) and the reten-tion capacity of H2S quickly decreases after a few cycles.
Others researchers have studied this oxidation at lower temper-atures with the intention of oxidise calcium sulphide and turning it into a mixture of calcium sulphate and calcium oxide, using for their works thermogravimetric analysis equipment or differential reactor equipment that requires small samples (<1 g) and small grain size with the main aim of measuring kinetic parameters [24-26].
Wu et al.  also used small amounts of calcium sulphide and claimed to have found a synergistic effect between H20 and 02 during high-temperature oxidation.
The effect of gaseous producís given off by a part of one particle into other parts of the same particle due to gaseous producís given off during CaS conversión ('intraparticle' reactions) has been dem-onstrated by some of these researchers despite using smaller grain sizes and smaller quantities of the substance [21,25]. Is evident that is possible the action of gaseous product released by one par-ticle on other parpar-ticle ('interparpar-ticle' reactions). Undoubtedly, highly significant 'intraparticle' and 'interparticle' effects would re-sult whenever larger grain sizes and larger quantities of substance are used to form a bed of considerable length compared with grain size.
In the study described herein, the product chosen for H2S absorption was dolomite as it works well under calcining (1173 K) and non-calcining(1123 K) conditions according to previ-ous studies by Adanez [18,19], Pinto et al.,  and Álvarez-Rodrí-guez and Clemente-Jul .
Furthermore, all the aforementioned studies on CaS oxidation have been carried out with purchased or prepared CaS. However, when dolomite is used as a desulphuring agent, the calcined prod-uct is a blend of CaO and MgO and forms a blend of CaS and MgO after its sulphurisation. Due to this fact, this product must be ob-tained in the laboratory itself because it is not a commercial product.
A large amount of product has also been used (100 g or 150 g of dolomite, bed lengths of 11.4cm and 17 cm, respectively) in a fixed-bed arrangement to more closely approximate industrial conditions because there are 'interparticle' reactions as well as 'intraparticle' reactions, since the gases given off by a particle can react with other particles encountered along the way. These reac-tions are minimised in thermogravimetric analysis carried out with very small mounts of substance.
The effect of grain sizes from 0.4 to 2 mm has also been studied to show the influence of intraparticle reactions.
Another problem is that the molar volume of calcium sulphate (46.0 cm3 m o r1) is higher than that of calcium sulphide (28.9 cm3 m o r1) or the initial calcium carbonate (36.9 cm3 m o r1) . Therefore, the pores of the particles produced by dolomite calcination could become clogged or covered during the oxidation reaction and eventually hinder complete oxidation [21,24-26].
Oxidation using oxygen can be formulated as reactions (2) and (3) (Table 1).
It is known that calcium sulphide can also be oxidised by carbón dioxide [25,26] and by water vapour [26,27]. In fact, various reac-tions have been proposed as (4)-(6) (Table 1). For instance, one of these reactions (4) is the inverse of COS absorption reaction by CaO, that takes place in the gas desulphurisation process. Other reaction is the inverse of H2S absorption by CaO (1).
These oxidant substances (02, H20 vapour and C02) are present in flue gases from combustión processes at various relative propor-tions, depending on the fuel used and the degree to which combus-tión is complete. For this reason, a gas blend that could be considered as an example of gases emitted by combustión pro-cesses has been used and the influence of each gas has been investigated.
In this investigation, which uses a relatively large amount of substance, several other factors were to be considered because, after the initial moments of oxidation, there are (at least superfi-cially) amounts of CaO that may react with some of the gases pres-ent in the gas stream or given off in the previous section of the sample, depending on its concentration and affinity, which also de-pends on temperature.
The temperature of gases that come into contact with the cal-cium sulphide has also been kept constant, but reactions (2) and (3) are very quick (see below) and exothermic. Therefore, the bed temperature increases considerably and consequently the reac-tions do no take place under isothermal condireac-tions.
If oxygen is present together with C02 and H20, any carbonyl sulphide formed by reaction (4) can react with oxygen according to the exothermic reaction (7) that modifies the gas composition and also generates more heat.
COS can also react with CaO by the reverse of reaction (4) and the newly formed CaS can react.
When water vapour is present, one of the possibilities is that hydrogen sulphide is formed by the reverse of reaction (1). This H2S can react with oxygen, leading to the exothermic reaction (8) (Table 1), which also modifies the gas composition and generates more heat.
Another possible reaction between COS and H20 is (9) (Table 1), a hydrolysis reaction that reduce the presence of COS.
lit-tle or no H2S in gases. However, COS is detected (and in especially case also CS2) which shows that reactions (4) and (12) can occur. The reaction (12) can be considered as the sum of reaction (4) plus reaction (13).
Another possible reaction considered by various authors and studied by Kamphuis et al.,  is (14) (Table 1). This is a reaction between solids and the author concludes that it takes place when a blend of these components is heated in an inert atmosphere at a temperature higher than 1100 K. Depending on the amounts ini-tially present, the reaction can attain near complete conversión.
During the oxidation of sulphurised dolomite, S02 is produced by reactions (2),(5) and (6). This gas cannot be emitted to the atmosphere, but can be used to produce sulphuric acid or can be converted in calcium sulphate by using methods similar to those used in the treatment of gases given off in combustión plants to genérate power. There are also several studies on S02 elimination such as  that uses a dual bed of potassium-containing coal pel-lets and calcium-containing pelpel-lets. Others use a product based on Fe/AC (AC: active carbon/coke) that can be regenerated  or an-other study that uses a Mo- and Co-doped V20/AC sorbent .
To simúlate a possible industrial application, this investigation used a recent calcium sulphide produced "in situ" (according the procedure described in Álvarez-Rodríguez and Clemente-Jul ) instead of puré calcium sulphide acquired from a supplier. For the production of this calcium sulphide, dolomite from the prov-ince of Granada, Spain, was used. Their X-ray diffractogram and analysis are shown in Fig. 1 and Table 2, respectively. The analysis show that their composition is very cióse to the mineral theoretical composition.
This dolomite can decompose completely at 850 °C and be transformed in calcium and magnesium oxides: Fig. 2 shows the thermogram for dolomite in a nitrogen atmosphere (40 cm3/min) with a temperature gradient of 10 °C/min up to 850 °C, followed by constant temperature thereafter. When the temperature reach 850° C continúes the lost of mass (C02 emission), but with the tem-perature stabilised at 850 °C, in about 200s the weigh stabilised and reach the theoretical for the total decomposition of the dolo-mite that is corroborated by X-ray diffraction. The thermobalance used was a Setaram-Labsys.
Granada dolomite analysis.
CaO MgO Fe203 MnO Ti02 Si02 A1203 K20 Na20 P205 Insoluble Loss on ignition
30.51 21.68 0.06 0.007 0.006 0.1 <0.1 <0.1 <0.1 <0.05
The calcined dolomite (a mix of CaO and MgO) is sulphurised using a blend of gases with H2S until the outlet gas composition stabilises and has virtually the same H2S content as the inlet gases. Conversión with regard to calcium with this procedure is about 97-99%.
This sulphidisation is carried out with the same equipment used for oxidation. In the case of oxidation, the inlet gas composition is changed after 'scrubbing' the reactor interior with puré nitrogen. The equipment used was a Kanthal vertical tube reactor with a length of 1.6 m and inner diameter of 27 mm which passes, in its central part, through a furnace with an inner length of 600 mm. This equipment was previously described by Adánez et al.
[17,19] and Álvarez-Rodríguez and Clemente-Jul .
To carry out the oxidation, the sample is initially stabilised at 850 °C or 700 °C using a nitrogen stream at the same velocity as the oxidising blend to control the furnace resistor temperature. A temperature of 850° was chosen because dolomite sulphidisation works very well at this temperature [17,19,28]. To study the influ-ence of temperature, other tests have been carried out using 700 °C .
Oxidation is then produced by injecting the oxidant blend (and modifying the nitrogen flow to maintain the total flow of gas) and the inlet gas velocity is kept at 10 1/min and 5 1/min (29.1 and 14.5 c m s- 1) , considered by various authors as a typical case of plug flow . All gases are controlled by specific mass flow con-trollers and water vapour is obtained by complete evaporation of a constant flow rate of water controlled by a mass flow controller
25 30 35 40 2Theta (Degrees)
5 E l-01 X T
90 80 70 60 50 40 30 20 10 0
-1 / 1 / V
/ * ' 11
0 1000 2000 3000 4000 5000 6000 7000 8000 9000 10000 Time s
Fig. 2. Thermogram of the dolomite used (- weight, — temperature).
and evaporator mixer. The certified deviations of the mass flow controllers (for flows measured under 75% of the fond scale) were lower than 0.3% of FS (±0.03 1/min for 10 1/min).
The gases are introduced at the top of the reactor to ensure that they move below through the material bed, oxidising the material. The gas temperature is controlled in the área where the gases come into contact with the sulphurised material. Oxidation is assumed to be complete when the S02 content of the outlet gas is less than 20 ppm.
Once oxidation is complete and after scrubbing with nitrogen to try to elimínate the physical absorbed gases, power to the furnace is cut off, the furnace is opened and the reactor is allowed to cool in a nitrogen atmosphere. Once cooled, the reactor is opened and the substance is collected.
The different gas blends used in the oxidation were: puré nitro-gen plus oxynitro-gen, nitronitro-gen plus carbón dioxide, nitronitro-gen plus water vapour and nitrogen with various levéis of carbón dioxide, water vapour and oxygen. The purpose of this choice was to analyse the possibility of using as oxidants the gases produced in combus-tión plants fired by various types of fuels.
The column of initial substance (dolomite) and later the bed to be oxidised (CaS plus MgO) in a fixed-bed arrangement is formed with 100 g or 150 g of granulometrically classified dolomite, as 0.4-0.5 mm, 0.71-1 mm or 2-2.5 mm to determine behaviour according to grain size. The use of 100 g leads to a bed length of 11.4 cm and 150 g leads to a bed length of 17 cm.
The oxidation gases given off by the reactor at the bottom flow through a coolant to sepárate any water used in the oxidant blend before the gases are analysed (for H2S, COS, S02 and C02) in a Var-ían CP-4900 Micro-GC chromatograph fitted with a 10 m Porabond O column module and Thermal Conductivity Detector that takes a sample every 5.7-6 min. There is also another DMD detector that is more sensitive to sulphur compounds and can be used to tray and detect other sulphur compounds, in very low quantities, such as CS2.
In experiments in which only oxygen (plus nitrogen) was used as an oxidant gas, oxygen was analysed using a TESTO 350 oxygen analyser. The oxidised sample was collected and analysed by X-ray diffraction (Phillips PX-1710) and wet chemical analysis to deter-mine CaS04 and CaS content.
Tests were carried out at atmospheric pressure with a slight overpressure of approximately 0.1 bar to simúlate the pressure re-quired for gas circulation. The total pressure was 0.11 MPa.
The conditions used in each test are shown in Table 2. Along with the tests Usted, other duplícate tests were carried out to en-sure results. The máximum deviation in chemical analysis is ±0.05 by valúes of the order of 50%, and ±0.01 by valúes lower than 1%.
3. Results and discussion
3.1. Oxidation with a blend ofN2 and 02 only
3.1.1. Influence of grain size and bed length
When operating as described in Section 2, dolomite sulphidisa-tion is virtually complete (97-99%) when a grain size of 2-2.5 mm is used. This grain size is the bigger size used in this work and by consequence the most difficult to sulphurise under different condi-tions. Fig. 3 shows the X-ray diffraction of sulphurised dolomite. The calcium sulphate or calcium oxide lines are absent and only de CaS (oldhamite) and MgO (periclase) lines can be seen.
Fig. 4 shows the plots of the variation of S02 content in the out-let gases with the time for various oxidation tests carried out using as oxidising gas a blend of 96% N2 and 4% 02 (tests 1, 6, and 11, Table 2). The gas velocity is of 29.1 cm s_ 1 and the sulphurised dolomite to be oxidised has grain sizes of 0.4-0.5 mm, 0.71-1 mm and 2-2.5 mm. The weight of the initial dolomite in the samples (previously to their calcination and sulfurisation) was 100 g (11.4cm bed length).
The analysis of oxidised samples is presented in the first three rows of Table 4. The table shows that residual CaS content in-creases with grain size, indicating that this factor has significant major influence. This occurs, as mentioned above, because the mo-lar volume of CaS04 is higher than that of the initial carbonate mol-ecule. The formation of this compound tends to clog pores and hinder oxidant penetration and therefore oxidation progress. This effect is more significant as grain size increases and becomes more difficult to reach the middle of the grain.
25 30 35 40
Fig. 3. Diffractogram of sulphurised Granada dolomite (O: oldhamite, P: periclase).
Fig. 4. S02 content in the outlet gases during oxidation at 850 °C, 4% 02,11.4 cm bed, 29.11 cm s ' gas velocity: tests 1 (A: 0.4-0.5 mm), 6 (•: 0.71-1 mm) and 11 (•:
In fine grain sizes, the large área increases the reaction rate and increases S02 production by oxidation and therefore CaO content. This S02 quickly comes into contact with the gas stream and is di-luted in this gas stream, thereby hindering adsorption by the outer layer of CaO, previously formed on others grains. In the larger grains and because oxidation should progress in more internal áreas of the grain, the S02 produced needs to pass through more layers of the grain to go out. Because oxygen and CaO are present in these áreas (previously oxidised), CaS04 may form as result, which tends to clog the pores due to a higher molar volume and stop any further oxidation earlier due to diffusion difficulties. This is a typical case of 'intraparticle' influence that increases with grain size.
This fact is not coincident with the fact than in the desulphuri-sation process the grain size may be bigger to obtain the máximum transformation rate of the calcined dolomite  using a fixed bed disposition. It is due that in the desulphurisation process there is not the problem of pore clogging into the calcined dolomite grain, but lower grain sizes results in greater grain packing in a compact bed of calcined dolomite grains, thus creating preferential paths for the gas and delaying H2S absortion. In the oxidation process the better grain size for the oxidation is the 0.4-0.5 mm, the smaller
used. In the desulphurisation process  the best gain size is 2 -2.5 mm, the bigger used.
To study the influence of bed length, a test was carried out with grain sizes of 2-2.5 mm (because it is the most sensitive size among those studies, due to containing more residual CaS) using 150 g of dolomite (17 cm bed length) instead of 100 g (Table 3). When compared with the 100 g test, a small increase in residual CaS is seen (4.55% vs. 4.32%); this reveáis that this parameter has little influence and shows that a little higher residual CaS content is obtained with higher bed lengths. This is due to the fact that the S02 gas produced (but diluted into the gas flow) circulates for longer among grains partially oxidised with CaO and has more opportunity to react with CaO and 02 to produce more CaS04, giv-ing rise to more pore clogggiv-ing. This is a typical case of 'interparti-cle' effect.
According to , reaction (14) (Table 1) can oceur at the tem-perature used (850 °C) but virtually No S02 (<20 ppm) is given off by the end of the test and residual CaS and CaS04 are present, showing that this reaction is virtually unimportant under the con-ditions used.
5 10 15 20 25 30 35 40 45 50 55 60 65 70 2Theta (Degrees)
25 30 35 40 2Thet¿ (Degrees)
Fig. 5. X-ray diffractogram of oxidized producís (4% 02)of test 1 (in top position) (0.4-0.5 mm), test 11 (inbottom position) (2-2.5 mm); A: anhydrite, L: lime, O: oldhamite
and P: periclase.
Test conditions for sulphunsed dolomite oxidation (nitrogen as balance gas).
Test 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19
Size ( m m ) 0.4-0.5 0.4-0.5 0.4-0.5 0.4-0.5 0.4-0.5 0.71-1 0.71-1 0.71-1 0.71-1 0.71-1 2-2.5 2-2.5 2-2.5 2-2.5 2-2.5 2-2.5 2-2.5 2-2.5 2-2.5
Bed length (cm) 11.4 11.4 11.4 11.4 5.7 11.4 11.4 11.4 17 11.4 11.4 11.4 11.4 17 11.4 11.4 11.5 11.5 11.5
Gas velocity (cms ') 29.11 29.11 29.11 29.11 29.11 29.11 29.11 29.11 29.11 29.11 29.11 14.55 29.11 29.11 29.11 29.11 29.11 14.55 29.11 Tempera. (°C) 850 850 850 850 700 850 850 850 850 850 850 850 850 850 700 850 850 850 950
o2 4 4
(%)lst No, lst No, 4 4 4 2 4
2 n d 4 2 n d 4
lst No 2nd 4
4 4 4 4 4 8 2-4
H20 (%)-7 7 -7 7 15.6 20 -7
-C 02 (%)-13 13 17 -13 13 7.8 -13 -21 -Table 4
Oxidation with a mix of 02 and N2: influence of grain size, temperature, bed length and oxygen partial pressure (oxygen content).
Test 1 6 11 14 15 5 19 12 16 17
Size ( m m ) 0.4-0.5 0.71-1 2-2.5 2-2.5 2-2.5 0.4-0.5 2-2.5 2-2.5 2-2.5 2-2.5
Bed length (cm) 11.4 11.4 11.4 17 11.4 5.7 11.4 11.4 11.4 11.4
Gas veloc. (cm s 29.11 29.11 29.11 29.11 29.11 29.11 29.11 14.55 29.11 29.11
4 4 4 4 4 4 4 4 8 2 Tempera. (°C) 850 850 850 850 700 700 950 850 850 850 CaO (%) 14.76 15.14 10.18 8.68 4.14 12.12 17.61 7.94 16.08 7.48
than for 0.71-1 mm, showing the effect of clogging o covering of pores. When gain sizes of 0.4-0.5 mm and 0.71-1 are compared, this does not occur and may be explained by greater packing and compactness in the case of the 0.4 mm grain size that causes more preferential pathways to circuíate the gas as shown in the case of sulphidisation [19,28].
3.1.2. ¡nfluence of temperature
Qiu et al.  concluded that temperature significantly affects CaS particle oxidation over the entire range of pressures tested in that study and that the level of CaS conversión to CaS04 increased notably with temperature between 700 °C and 900 °C. Test 15 (2-2.5 mm, 4% 02, 96% N2, 29.1 l c m s "1 gas velocity), Table 4, was car-ried out at a gas inlet temperature of 700 °C instead of 850 °C (test 11) and showed that residual CaS increased notably (20.07% vs. 4.32%) and that CaS04 content is lower (47.58% vs. 58.5%). This clearly shows the influence of temperature.
Another test (test 5, Tables 3 and 4) with 50 g and a particle size of 0.4-0.5 mm showed how a high residual amount of CaS (5.57%) is left behind despite lower grain size and shorter bed length. This amount was significantly higher than in the test at 850° with 100 g of dolomite (0.45%) also shown in Table 4.
These results are consistent with the observations by García-Calzada et al.  on the calcium sulphide stabilisation due to air heating. Those authors concluded that the best range of temper-ature was between 800 °C and 870 °C. Those authors concluded that the best range of temperatures was between 800 °C and 870 °C. They claim also a relationship between a high conversión to sulphate and virtually zero emission of S02, but this is not in our case.
3.1.3. ¡nfluence of gas velocity for oxidation and concentration of 02
All factors that favour contact between S02 produced by oxida-tion reacoxida-tions (principally reacoxida-tion (2)) and CaO previously pro-duced lead to an increase in residual CaS due to increased formation of surface CaS04 that increased the effect of pore clog-ging due to the clogclog-ging effect of this compound. Table 4 shows the results of various tests with two oxidation gas velocities and three oxygen concentrations. When the results shown in Table 4 are compared, an increase in residual CaS can be seen at lower velocities (test 12 vs. test 11) and at lower oxygen concentrations (test 11 vs. test 16). These results are consistent with  who showed that increased 02 partial pressure results in increased oxi-dation rate, at least initially.
Comparing test 11 with test 12 in Table 4, lower gas velocity can also be seen to reduce CaO/CaS04 ratio, showing how the contact time between gas and solid enhances sulphate formation.
Fig. 6 contains plots for S02 reléase at oxygen concentrations of 4% and 8% in the oxidation gas under otherwise equal conditions (gas velocity 29.11 c m s ~ \ grain size 2-2.5 mm and bed length 11.4cm). Oxidation rate increases notably at higher oxygen con-tent or concentration levéis, thereby increasing the amount of S02 in the outlet gases (higher área), consistent with the higher CaO content in the end product.
This effect of gas velocity cannot be clearly separated from the temperature effect in these test carried out with a large amount of substance. This is because any oxidation reactions (2) or (3) are highly exothermic and an increase in gas velocity at the same oxy-gen concentration (4%) increased 02 availability per unit time and increases temperature. The same occurs when 02 content or con-centration increases and the inverse occurs when it decrease. Qiu et al.  has suggested that this influence of heat generated by exothermic oxidation of CaO explain some observations in virtually 'intraparticle' reaction as they use a very small amount of sub-stance. This becomes much more important when a large amount of substance is involved.
3.1.4. Behaviour of 02 during oxidation
02 reacts with CaS very quickly and the reactor outlet gases contain virtually No 02 in within a few minutes of oxidation, even when 8% 02 is used.
Fig. 7 shows the trend over time of the oxygen concentration in the reactor outlet gas when using grain sizes of 2-2.5 mm, 8% 02 and a gas velocity of 29.11 c m s- 1 (test 16, Table 3). Plots are shown for 4% 02 and two gas velocities (29.11 c m s- 1 (test 11) and 14.55 cm s_ 1 (test 12) are used.
In the first few minutes (more minutes at lower oxygen con-centration and lower gas velocity), there is virtually no oxygen in the outlet gas. It is also evident that its content will subse-quently increase until it virtually reaches the initial concentration at the end of the tests when S02 content is very low (<20 ppm). This is due to the fact that at higher oxygen concentration and higher gas velocity there are more supply of oxygen by time unit, and by this is more difficult for all the oxygen to react and this element will appear earlier in the outlet gases. This may be important when comparing the action of oxygen with other oxi-dants, such as C02 and H20, that react more slowly. This is dis-cussed below.
100 150 200 250 minutes
100 150 minutes
Fig. 7. 02 trend at 850 °C and grain size 2-2.5 mm; tests 16 (O: 8% 02, 29.11 cm s"1), 11 (•: 4% 02, 29.11 cm s"1) and 12 (•: 4% 02,14.5 cm s"1).
3.2. ¡nfluence of other oxidant gases: C02 and H20
3.2.1. Oxidatíon by C02
Anthony et al.  established that C02 reacts with CaS to pro-duce S02 and CO, but little or no COS. To clarify the C02 effect, two tests have been carried out: one with C02 (21%) and N2 (test 18, Ta-ble 3), and another with C02 (17%) and N2 only at the beginning and later with C02, N2 plus 4% 02 (test 4).
When only C02 (21%) is used (test 18 in Table 3) in a sulphured sample of 2-2.5 mm grain size, 14.55 c m s- 1 gas velocity and 11 cm bed thickness, the gases emitted over time are shown in Fig. 9. With respect to COS, initially there is great COS reléase, but this quickly decreases. With respect to S02 initially is a little re-léase that initially decreases slowly over time and later increases until a constant level of approximately 1000 ppm is attained.
From the different reactions that can be considered, it is obvious that reaction (4) is initially important but reaction (5) is later dom-inant. In any case, COS released tends to stabilise around 20 ppm.
There is no clear evidence that reactions (15) and (16) produc-ing calcium carbonate or calcium sulphate take place. The X-ray diffractogram for this sample (Fig. 9) shows no calcium carbonate or calcium sulphate peaks (these producís are highly crystalline and readily detected). In the chemical analysis of the end product, the amount of calcium sulphate detected after more than 6 h of treatment is only 0.24%, very low compared to the amount of cal-cium oxide (8.95%). The peak of this CaO, which is much less crys-talline than other compounds considered is easily detected in the diffractogram.
Initially, on the action of C02 when 1465 ppm of COS is de-tected, a mínimum amount of CS2 is also detected by using a DMD detector, a detector specifically for sulphur compounds (this low amount of CS2 cannot be detected with the commonly used TCD detector). Latter, this peak of CS2 is less visible when the amount of COS present is 480 ppm and after it cannot be observed. This means that reactions (12) or (13) are possible, bearing in mind that reaction (12) can be considered the sum of reactions (4) plus (13).
The C02 concentration used is not a determining factor for this behaviour because the content or concentration of this compound in the initial gas is 21% and little is consumed, which means that the C02 concentration is virtually steady al all reacting points and at all times. The most notable difference between the initial and subsequent moments is that the sample surface is initially
composed almost entirely of CaS and afterwards CaO is present on the grain surface, at least partially.
This behaviour could be attributed to a chain of reactions: ini-tially, reactions (4) and (12) take place in competition with reac-tion (5) while only CaS is present on the surface. Later, when CaO has also formed, part of the COS (and CS2) reacts with CaO to pro-duce new CaS according to the reverse of reaction (4). This newly formed CaS reacts according to (4) and (5) and by successive reac-tions, the amount of COS produced is notably reduced and tends to steady state. The same occurs with COS released from the inner layers of a grain. This COS must go through outer layers with CaO (this effect is more significant at larger grain sizes) and reacts according to the reverse of reaction (4).
The rate of CaS decomposition due to reaction with C02 at 850 °C is very small (Fig. 8). Although it would be possible accord-ing to Anthony et al.  to completely oxidize CaS because there is virtually no covering or clogging of pores because no calcium carbonate or calcium sulphate is being formed, this would take a long time. In the case considered and assuming a stabilised pro-duction of approximately 1000 ppm of sulphur compounds (S02 plus COS) at gas velocity of 51/min, this is equivalent to 0.0134 mol/h. Since the CaO involved in the test is 0.544 mol (100 g of dolomite), the complete conversión would take 40.6 h (if the reléase rate does not change).
160 200 240 minutes
Fig. 8. COS and S02 content in the outlet gases during oxidation in test 18: oxidation with 21% C02, grain size 2-2.5 mm, 850 °C, COS (•), S02 (•
10 25 30 35 40 45
Fig. 9. X-ray diffractogram of the product of test 18; oxidation with 21% of C02, 79% N2; L: lime, O: oldhamite, P: periclase.
4 the complete conversión would take about 20 h and in the test 18 would take 40 h (if the reléase rate does no change at times longer that the used in the tests).
3.2.2. Oxidation by H20
Wu  found that H20 vapour can react directly (in absence of oxygen) with CaS and produces S02, H2 and a negligible amount of H2S and No CaS04.
Test 10 was performed using only nitrogen and 20% H20 (for 110 min) and show an initially large reléase of H2S that quickly dropped to steady state at about 370 ppm and an initially low re-léase of S02 that also tended to reach steady state at approximately 540 ppm (Fig. 10).
Reactions (6) and the reverse of reaction (1) are different ways to oxidise calcium sulphide; one produces S02 and the other H2S. This means that reactions (6) and the reverse of reaction (1) are competing reactions. Where CaO is not present, the reverse of reac-tion (1) is more important and H2S is released throughout the en-tire CaS column because the reaction is not very 'extensive' (unlike what occurs with oxygen) and does not consume all the water va-pour introduced, but rather only a very small proportional part. When some CaO has already been formed, H2S is adsorbed on
CaO to restore CaS according to reaction (1). CaS is then oxidised again by H20. The result is a drop in the amount of H2S produced and an increase in S02 until steady state is achieved. This steady state is maintained for a long time because oxidation with water under the conditions used is not very active. This phenomenon also occurs inside the grain when H2S produced inside the grain must go through the previously formed CaO layer.
As occurs with the case of C02, during oxidation by water va-pour, the oxidation rate is very low under the conditions used (approximately 900 ppm of sulphur compounds are released).
After 110 min, 4% 02 is introduced (in addition to water vapour) and the oxidation reaction speeds up; 240 min later, oxidation stops (S02 concentration in the gas released is 18 ppm) and the chemical analysis gives 38% residual CaS, showing that more pore clogging or covering has occurred. This is important and is further discussed in Section 3.2.3.
3.2.3. Oxidation with a blend of N2 plus 02, C02 and H20
12000- 10000-Q. Q.
^ * = * - * - t - t - l 1 1 1 1 1 1 1 1 1 * 1 1 V « >< M i»
50 100 150
Fig. 10. H2S and S02 trend in test 10 (oxidation with 20% H20, grain size 0.71-1 mm, 850 °C) S02 (•), H2S (•).
76% N2, using a gas temperature of 850 °C, gas velocity of 29.11 c m s ~ \ 100 g of dolomite and the three grain sizes raen-tioned above (tests 2, 7, 8 and 13)
As discussed previously, the presence of C02 and H20 will lead to the formation of COS and H2S as well as S02 and CO. However, these oxidant compounds do no react extensively and are not con-sumed in the initial CaS bed área and therefore act over the entire length of the bed. Oxygen, by the contrary, is consumed in the first part of the CaS bed and need time to be detected at the end of the bed, especially if the oxygen concentration is not very high. As a re-sult, COS and H2S initially appears in the outlet gases and tend to disappear in this gas over time for reasons discussed in previous points and also because when appears any oxygen in the lower part of the bed oxidises any COS, CO and H2S according to reactions (7) and (8). Initially, the Figs. 11 and 12 (test 13, Table 3) show that the H2S concentration is approximately 1000 ppm and the COS is virtually invisible in this figure because its content is about 5 ppm. Both compound decreases rapidly their presence and prac-tically disappears at 20 min. The low level of COS can be explained by its reaction with the water introduced (9).
The chemical analysis results listed in Table 5 show that resid-ual CaS is higher than in previous cases when only a blend of oxy-gen and nitrooxy-gen is used (all other conditions being equal) as can be seen comparing test 2 in Table 5 with test 1 in Table 4; test 7 in Table 5 with test 6 in Table 4 and test 13 in Table 5 with test 11 in Table 4. The influence of grain size is also more important than when only oxygen is used as an oxidant. CaO content is higher than when only nitrogen and oxygen are used, although the cal-cium sulphate content is lower.
A comparison was performed with grain size of 0.4-0.5 mm un-der conditions of oxygen and nitrogen only (test 1 in Table 4) and under conditions of a blend with the same oxygen concentration (4%) but with water vapour and carbón dioxide (test 2 in Table 5). This comparison showed that the CaO content in the product was higher when water and carbón dioxide were used (19.17% vs.14.76%) despite higher residual CaS content (0.83% vs. 0.45%). This finding is not consistent with  on this point.
Using higher grain sizes (2-2.5 mm), residual CaS under condi-tions of a blend with oxygen (4%), water vapour and carbón dioxide is much higher (23.58%, test 13 in Table 5) than when only nitrogen
80 100 120 minutes
300-0 2300-0 4300-0 6300-0 8300-0 1300-0300-0 12300-0 14300-0 16300-0 18300-0 2300-0300-0 minutes
Fig. 12. S02, H2S, and COS evolution in test 13, enlargement of Fig. 12 (oxidation mix: H20, C02 and 02, grain size 2-2.5 mm, 850 °C). S02 (•), H2S (•), COS (•) 12H2S.
Oxidation with a mix of 02) 7% H20,13% C02 and N2 as balance gas: influence of grain size and oxygen partial pressure (oxygen content).
2 7 13 8
0.4-0.5 0.71-1 2-2.5 0.71-1
Bed length (cm)
11.4 11.4 11.4 11.4
29.11 29.11 29.11 29.11
(cm s ') o2
4 4 4 2
(%) Tempera. (°C)
850 850 850 850
19.17 21.75 11.57 18.40
50.78 44.44 33.50 46.24
(%) CaS (%)
0.83 3.26 23.58 5.46
0.378 0.489 0.345 0.398
567 .¥ 504
-£ 252 £ 189
Uf-A^.0 5 10 15 20 25 30 35 40 45 50 55
60 65 70
•£ 567 ¿ 504
t 441 .= 378 | 315 Z 252 | 189 £ 126 ¿ 63
, Mi f . i n A l ' . ^ I . J
10 15 20 25 30 35 40 45 50 55 60 65 2Theta (Degrees)
Fig. 13. X-ray difractograms of the oxidation producís of tests 2 (0.4-0.5 mm) (in top) andl3 (2-2.5 mm) (in bottom), with a mixof 4% 02,13%C02 and 7% H20, 850 °C; A:
and oxygen are used (4.32%, test 11 in Table 4) due to more pore clogging caused by larger grain size. The CaO content is slightly higher than when only nitrogen and oxygen are used (11.57% vs. 10.18%).
The CaS/CaS04 ratio is higher in all grain sizes when used the mix of water vapour, carbón dioxide and oxygen compared to tests conducted with the same temperature, bed length and gas velocity, but with only N2 and 4% 02 (tests 2, 7 and 13 in Table 5 compared respectively with tests 1, 6 and 11 in Table 4).
This contradicts studies by Wu  who defended a synergistic action of H20 and 02 during CaS oxidation. Wu's study was carried out with a small amount of substance (60 mg). According to that study, water vapour was able to achieve greater penetration; moreover, CaO formation (instead CaS04) would facilítate oxygen access.
In the present study conducted with a large amount of sub-stance, one explanation is that the innermost pores created by H20 are used by the oxygen and S02 blend previously produced to yield calcium sulphate with CaO. This increased the possibility of earlier, more substantial, pore clogging and will therefore leave more residual CaS.
Fig. 13 shows the X-ray diffractograms of the two extreme cases (test 2 and 13, 0.4-0.5 mm and 2-2.5 mm). The large amount of residual CaS in the case of the larger size is obvious.
Test 9 (Table 3) was carried out using 150 g instead of 100 g, which has little effect on residual CaO as discussed previously. In this test, however, the water vapour content is higher (15.6%) and the carbón dioxide content is lower (7.8%), but the oxygen con-centration remains steady (4%) as compared with test 7 (Tables 3 and 5). The results of this test (no shown in the tables) are: Resid-ual CaS: 8.58%, CaO: 20.3% and CaO/CaS04 ratio 0.508. ResidResid-ual CaS increases by 8.58% compared with 3.26%, showing the negative ef-fect of water vapour, because carbón dioxide has been reduced. The CaO content is of 20.3% a little lower than in test 7 (21.75%). The CaO/CaS04 ratio was increased by 0.508, higher than in the test conducted using the same grain size and temperature, but with only 7% water vapour: 0.489 in test 7, Table 5.
1. The most efficient oxidant for CaS is 02. H20 and C02 can also oxidise CaS, but at a much slower rate than 02.
2. When H20 vapour is mixed with N2 and 02, a higher amount of residual CaS is produced than with the N2 and 02 blend alone, but increases CaO content.
3. Grain size is a key parameter for the control of residual CaS under any conditions (fixed bed arrangement) due to problems of pore clogging. The best grain size is the smaller used: 0.4-0.5 mm. In the desulphurisation process is the contrary to obtain the best results, the better grain size is the bigger used 2-2.5 mm because there is not a problem of pore clogging. 4. Higher 02 concentrations in the oxidation gas produce lower
amounts of residual CaS.
5. Less residual CaS is produced at 850 °C than at 700 °C. More CaS04 conversión, more pore clogging and more residual CaS occurs at a lower temperature.
6. Increased bed length moderately increases residual CaS. 7. C02 used alone produces a notable amount of COS and a very
small amount of CS2 at the start of oxidation but these com-pounds tends to quickly decrease due to a chain of reactions with produced previously CaO and COS tends to be much lower than S02 production.
8. Water vapour used alone produces a notable amount of H2S at the start of oxidation, but the latter compound tends to
decrease quickly due to a chain of reactions with previously produced CaO and tends to be equal to S02 production.
The authors would like to thank the European Commission-DG Research, Research Fund for Coal and Steel (RFC-CR-04006) for supporting this study.
The authors would also like to thank UPM - R05/11205(RFC M0500204145) and UPM - CCG06-UPM/TQ-351 (RFC M0700204178) for supporting this line of investigation of the re-search group.
 Westmoreland PR, Gibson JB, Harrison DP. Comparative kinetics of high temperature reaction between hydrogen sulphide and selected metal oxides. Environ Sci Technol 1997;11:488-91.
 Christoforu SC, Efthiniadis EA, Vasolos I. Sulphidation of mixed metal oxides in a fluidized bed reactor. Ind Eng Chem Res 1995;34:83-93.
 Tomás-Alonso F, Palacios JM. Synthesis and surface properties of zinc ferrite spices in supported sorbents for hot-coal gas desulfurization. Fuel Process Technol 2004;80:191-203.
 Pineda M, Palacios JM, Alonso L, García E, Moliner R. Performance of Zn oxide based sorbents for hot-coal gas desulfurization. Fuel 2000;79:885-95.  Alonso L, Palacios JM, Moliner R. The performance of some Zn based
regenerable sorbents in hot coal gas desulphurization long-term using graphite as a pore-modifier additive. Energy Fuels 2001;15:1396-402.  Ahmed MA, Alonso L, Palacios JM, Cilleruelo C, Abanades JC. Structural changes
in Zn derrites as regenerable sorbents for hot coal gas desulphurization. Solid State Ion 2000;138:51-62.
 Alonso L, Palacios JM, García E, Moliner R. Characterization of Mn and Cu oxides as regenerable sorbents for hot coal gas desulphurization. Fuel Process Technol 2000;62:31-44.
 García E, Palacios JM, Alonso L, Moliner R. Performance of Mn and Cu mixed oxides as regenerable sorbents for hot coal gas desulfurization. Energy Fuels 2000;14:1296-303.
 Alonso L, Palacios JM. Performance and recovering of a Zn-doped Mn oxide as a regenerable sorbent for hot-coal gas desulfurization. Energy Fuels 2002;16:1550-6.
10] Pan YG, Perales JF, Velo E, Puigjaner L Kinetic behaviour of iron oxide sorbent in hot gas desulphurization. Fuel 2005;84:1105-9.
11] Risnes H, Fjellerup J, Henriksen H, Moilanen A, Norby P, Papadakis K, et al. Calcium addition in straw gasification. Fuel 2003;82:641-51.
12] Lin S, Harada M, Suzuki Y, Hatano H. Continuous experiment regarding hydrogen production by coal/CaO reaction with water vapour (I) gas producís. Fuel 2004;83:869-74.
13] Adánez J, Diego LF, García-Labiano F, Abad A. Kinetics of H2S reaction with calcined calcium-based sorbents. Energy Fuels 1998;12:617-25.
14] García-Labiano F, Adánez J, Abad A, Diego LF, Gayan P. Effect of pressure on the sulfidation of calcined calcium based sorbents. Energy Fuels 2004;18:761-9. 15] Adánez J, Abad A, Diego LF, García-Labiano F, Gayan P. Direct sulphidation of
half-calcined dolomite under pressurized conditions. Ind Eng Chem Res 2004;43:4132-9.
16] Diego LF, García-Labiano F, Adánez J, Palacios JM. Factors affecting the H2S reaction with non-calcined limestones and half-calcined dolomite. Energy Fuels 1999;13:146-53.
17] Abad A, Adánez J, García-Labiano F, Gayan P. Hot coal-gas desulphurization with calcium based sorbents in a pressurized moving-bed reactor. Energy Fuels 2004;18:1543-54.
18] Diego LT, Abad A, García-Labiano F, Adánez J, Gayan P. Simultaneous calcinations and sulfidation of calcium-based sorbents. Ind Eng Chem Res 2004;43:3261-9.
19] Adánez J, Abad A, García-Labiano F, Diego LF, Gayan P. H2S retention with Ca-based sorbents in a pressurized fixed-bed reactor: application to moving-bed design. Fuel 2005;84:533-42.
20] Pinto F, Lopes H, André RN, Gulyurtlu I, Cabrita I. Effect of catalysts in the quality of syngas and by-products obtained by co-gasification of coal and wastes. 2: Heavy metáis, sulphur and halogen compounds abatement. Fuel 2008;87:1050-62.
21] García-Calzada M, Marbán G, Fuertes AB. Decomposition of CaS particles at ambient conditions. Chem Eng Sci 2000;55:1661-74.
22] Brooks MW, Lynn S. Recovery of calcium carbonate and hydrogen sulfide from waste calcium sulfide. Ind Eng Chem Res 1997;36:4236-42.
23] Schwerdtfeger K, Brin I. Problems in hot desulfurization of coal gas with lime. Erdoel Kohle Erdgas, Petrochem 1993;46:103-10.
24] Qiu K, Lindqvist O, Mattison T. Oxidation behaviour of desulphurization residues from gasification and fuel-rich combustión. Fuel 1999;78:225-31. 25] OJu K, Anthony EJ, Jia L. Oxidation of sulfidized limestone under the conditions
 Anthony EJ, Jia L, Qiu K. CaS oxidation by reaction with C02 and H20. Energy Fuels 2003;17:363-8.
 Sh Wu, Azhar Uddin Md, Nagamine Sh, Sasoaka E. Role of water vapour in oxidative decomposition of calcium sulphide. Fuel 2004;83:671-7.
 Álvarez-Rodríguez R, Clemente-Jul C. Hot gas desulphurization with dolomite sorbent in coal gasification. <http://dx.doi.Org/10.1016/j.fuel.2008. 07.010>.
 Kamphuis B, Potma AW, Prins W, Van Swaaij PM. The reductive decomposition of calcium sulphate-I. Kinetics of the apparent solid-solid reaction. Chem Eng Sci 1993;48:105-16.
 Bueno-López A García-García A. Combined S02 and N02 removal at modérate temperature by a dual bed of potassium-containing coal-pellets and calcium-containing pellets. Fuel Process Technol 2005;86:1745-59.
[31 ] Ma J, Liu Z, Zhu Z. A regenerable Fe/AC desulfurizer for S02 adsorption at low temperatures. Appl Catal B 2003;45:301-9.
 XingX, Liu Z, YangJ. Mo and Co doped V205/AC catalyst-sorbents for flue gas S02 removal and elemental sulphur production. Fuel 2008;87:1705-10.  García-Calzada M, Marbán G, Fuertes AB. Stability and oxidative stabilisation